• Especially advantage is derived when used in conjunction with silica fume as silica fume greatly increase water demand to make mix workable.
|Loss of workability of
concrete with time of concretes: (A)
water/cement ratio=0.58 without admixture; (B)
water/cement ratio=0.47 with superplasticizer
Naphthalene based superplasticizer was used in this example; two concrete samples are compared here one without admixture and other with superplasticizers. It can be noticed that loss of workability occurs much quicker in concrete having superplasticizers; but obviously, concrete with superplasticizers has lower water/cement ratio which will yield higher strength.
Because duration is a prime parameter for effectiveness of superplasticizers, it is advantageous to introduce superplasticizers into the concrete mix in two stage, or even more, operations. Such re-dosage or repeated addition is possible when concrete is delivered to construction site by agitator truck. If it is required to restore workability by re-dosage after some period of actual mixing, adequate amount of super plasticizers should be added to act on both hydration products of cement and cement particles that are not hydrated yet. Therefore a small re-dosage of superplasticizers will not work, higher re-dosage is necessary.Though repeated addition of superplasticizers to concrete mix is found advantageous in respect of improvement of workability, they may increase segregation and bleeding. Other possibilities are to alter in amount of air entrainment and set retardation. Besides these side-effects, the second dosage applied to restore workability may reduce it at a faster rate than that of initial rate. Considering this effect, it is preferred to apply re-dosage immediately before placing and compaction of concrete.Following figure shows an effect of applying a re-dosage of superplasticizers (naphthalene based) on workability for a mix having water/cement ration of 0.50; the first dosage are followed by three re-dosage,each dosage were identical i.e. 0.4% of solids by weight of cement. The amount of Super plasticizer that is required to include in mix to restore workability change with temperature and water/cement ratio. More quantity of superplasticizer is required as temperature raise within the range of (30~60)0
• Increasing amount of superplasticizers
• Application of any suitable retarder
• Re-dosing of superplasticizers at designed time intervals
• Selecting admixture having coarser grain
• Blending with admixtures or polymers (water soluble)
Retempering of concrete to retain slump is examined in many research, the effect of retempering at different water/cement ratios of concrete are examined with concrete containing0.5% superplasticizers by mass of cement having water/cement of 0.5,0.6 and 0.7. At lower water/cement ratios, the retempering
effect is found more pronounced in respect of slump increase. Though rate of loss of slump is identical for four samples, slump retention is found higher at concrete of low water/cement ratio. Again it is found that concretes having low water/cement ratio have higher strength than that is not retempered.
Requirements of superplasticizers
• They have successfully used with flyash in concrete mix
• Special advantage is derived when used in conjunction with silica fume as silica fume greatly increase water demand to make mix workable. But if re-dosages is required, the higher quantity of superplasticizers is required than concrete not containing silica fume.
• Superplasticizers have no influence on
• Modulus of elasticity
• Resistance against freezing and thawing
• No effect on durability of concrete (in present state of knowledge); particularly for air-entraining agents, special care should be taken as sometimes it is reported that entrained air has reduced by superplasticizers.Slump loss depends on following factors:
• Amount and type of superplasticizers
• Amount and type of cement
• Time of application of superplasticizers
• Mix criteria
• Existence of admixture except superplasticizers.
Chemistry of slump loss:
During the period of slump loss, the tricalcium aluminate of cement reacts with gypsum which yields product having crystalline structure and distributed within mass. Thus reactions occur in aluminate phase have important influence on concrete workability. It is reported that when superplasticizer is added to concrete reaction between this phase and gypsum are enhanced; this rate, in addition, may also enhanced when excess sulfate is available in concrete.
Young conducted experiments on individual phase of cement; slump loss was examined under
• 30% gypsum + Tricalcium Aluminate
• Tricalcium Aluminate + Tricalcium Silicate + Gypsum
• Tricalcium Silicate system
Slump loss was not found in C3A and gypsum system. However a relation between slump loss and C3S phase was established. To gain a particular slump, higher amount of silicate phase were essential, again greater loss of slump was related to this phase. Thus it seems to restore tendency of flocculation with restoration of change interactions between grains of C3S by formation of hydration coatings. When re-dosages of superplasticizers are applied, these charges are neutralized and thereby restore fluidity. However continuation of hydration will result slump loss. Any retarder exist in concrete to retard hydration of C3S are desired to stave off the commencement of quick loss.
Hanna et al. developed a procedure to explain behavior of cements with SNF. Following evaluation is proposed to define fluidity in respect of aluminate phase of cement paste: